Crystal chemistry and physical properties of the A<sub>2</sub>M<sub>3</sub>(H<sub>2</sub>O)<sub>2</sub>[B<sub>4</sub>P<sub>6</sub>O<sub>24</sub>(OH)<sub>2</sub>] (A = Cs, Rb; M = Ni, Cu, (Ni, Fe)) borophosphate family.
Shvanskaya, Larisa; Yakubovich, Olga; Melchakova, Lyubov; Ivanova, Anna; Vasiliev, Alexander; Dalton transactions (Cambridge, England : 2003) 48 (2019) 8835–8842; doi:10.1039/c9dt00564a

data_7700020
_publ_section_title
;
 Crystal chemistry and physical properties of the
 A<sub>2</sub>M<sub>3</sub>(H<sub>2</sub>O)<sub>2</sub>[B<sub>4</sub>P<sub>6</sub>O<sub>24</sub>(OH)<sub>2</sub>]
 (A = Cs, Rb; M = Ni, Cu, (Ni, Fe)) borophosphate family.
;
_journal_issue                   24
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              8835
_journal_page_last               8842
_journal_paper_doi               10.1039/c9dt00564a
_journal_volume                  48
_journal_year                    2019
_chemical_formula_moiety         'B8 Fe H12 Ni5 O56 P12,0.52(Rb2), 2.96(Rb)'
_chemical_formula_sum            'B8 Fe H12 Ni5 O56 P12 Rb4'
_chemical_formula_weight         2057.50
_chemical_name_common            'Rubidium nickel-iron borophosphate'
_chemical_name_systematic
;         
Dirubidium Diaquatrinickel-iron 24-oxodihydroxotetraborohexaphosphate(V)borophosphate
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           61
_space_group_name_Hall           '-P 2ac 2ab'
_space_group_name_H-M_alt        'P b c a'
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.4599(4)
_cell_length_b                   12.2035(4)
_cell_length_c                   19.9085(6)
_cell_measurement_reflns_used    2944
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.159
_cell_measurement_theta_min      2.912
_cell_volume                     2298.31(14)
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_molecular_graphics    'DIMOND (Brandenburg, 2006)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 16.0630
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Xcalibur, Sapphire3'
_diffrn_measurement_method       \w
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0875
_diffrn_reflns_av_unetI/netI     0.0499
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            15465
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        24.976
_diffrn_reflns_theta_max         24.976
_diffrn_reflns_theta_min         2.910
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    7.096
_exptl_absorpt_correction_T_max  0.696
_exptl_absorpt_correction_T_min  0.399
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Numerical absorption correction based on gaussian integration over
            a multifaceted crystal model
;
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.973
_exptl_crystal_description       'plateled column'
_exptl_crystal_F_000             1988
_exptl_crystal_size_max          0.093
_exptl_crystal_size_mid          0.056
_exptl_crystal_size_min          0.028
_refine_diff_density_max         0.761
_refine_diff_density_min         -0.808
_refine_diff_density_rms         0.148
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.315
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     196
_refine_ls_number_reflns         2023
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.314
_refine_ls_R_factor_all          0.0720
_refine_ls_R_factor_gt           0.0618
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0140P)^2^+14.0253P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0943
_refine_ls_wR_factor_ref         0.0972
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1808
_reflns_number_total             2023
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9dt00564a3.cif
_cod_data_source_block           shelx
_cod_depositor_comments
'Adding full bibliography for 7700020--7700022.cif.'
_cod_database_code               7700020
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.558
_shelx_estimated_absorpt_t_max   0.826
_shelx_res_checksum              64507
_shelx_hkl_checksum              78534